Low-temperature behaviour of K<sub>2</sub>Sc[Si<sub>2</sub>O<sub>6</sub>]F: determination of the lock-in phase and its relationships with fresnoite- and melilite-type compounds.
Hejny, C.; Bindi, L.; Acta crystallographica Section B, Structural science, crystal engineering and materials 73 (2017) 923–930; doi:10.1107/S2052520617010241

data_2311788
_publ_section_title
;
 Low-temperature behaviour of
 K<sub>2</sub>Sc[Si<sub>2</sub>O<sub>6</sub>]F: determination of the
 lock-in phase and its relationships with fresnoite- and melilite-type
 compounds.
;
_journal_coeditor_code           DK5057SUP1
_journal_issue                   'Pt 5'
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              923
_journal_page_last               930
_journal_paper_doi               10.1107/S2052520617010241
_journal_volume                  73
_journal_year                    2017
_chemical_formula_moiety         'F18 K O108 Sc18 Si36, 35(K)'
_chemical_formula_sum            'F18 K36 O108 Sc18 Si36'
_chemical_formula_weight         5298.12
_space_group_crystal_system      monoclinic
_space_group_IT_number           10
_space_group_name_Hall           '-P 2y'
_space_group_name_H-M_alt        'P 1 2/m 1'
_audit_creation_method           SHELXL-2013
_audit_update_record
;
2017-08-09 # Formatted by IUCr publCIF

;
_cell_angle_alpha                90
_cell_angle_beta                 90.000(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   26.785(3)
_cell_length_b                   8.2451(16)
_cell_length_c                   26.824(3)
_cell_measurement_reflns_used    589
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      15.4
_cell_measurement_theta_min      4.2
_cell_volume                     5923.9(15)
_computing_cell_refinement       '<i>CrysAlis</i> (Oxford Diffraction, 2006)'
_computing_data_collection       '<i>CrysAlis</i> (Oxford Diffraction, 2006)'
_computing_data_reduction        '<i>CrysAlis</i> (Oxford Diffraction, 2006)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 2001)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS-2013 (Sheldrick, 2013)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.960
_diffrn_measurement_device_type  'Oxford Xcalibur 3'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.032
_diffrn_reflns_av_unetI/netI     0.0114
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.960
_diffrn_reflns_number            28536
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.960
_diffrn_reflns_theta_full        25.240
_diffrn_reflns_theta_max         27.996
_diffrn_reflns_theta_min         3.042
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    2.751
_exptl_absorpt_correction_T_max  0.995
_exptl_absorpt_correction_T_min  0.994
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(<i>ABSPACK</i>; Oxford Diffraction, 2006)'
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    2.970
_exptl_crystal_description       block
_exptl_crystal_F_000             5184.0
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.070
_exptl_crystal_size_min          0.060
_exptl_transmission_factor_max   0.945
_exptl_transmission_factor_min   0.815
_refine_diff_density_max         0.560
_refine_diff_density_min         -0.936
_refine_diff_density_rms         0.116
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.281
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1087
_refine_ls_number_reflns         14668
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.281
_refine_ls_R_factor_all          0.0327
_refine_ls_R_factor_gt           0.0312
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0561P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1010
_refine_ls_wR_factor_ref         0.1011
_reflns_Friedel_coverage         0.000
_reflns_number_gt                11412
_reflns_number_total             14668
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            dk5057sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        5924.1(15)
_cod_original_sg_symbol_H-M      'P 2/m'
_cod_database_code               2311788
_publcif_datablock.id            {9c7527d8-f9a1-4280-9998-e33738fbf57e}
_shelxl_version_number           2013-4
_shelx_res_checksum              41971
_shelx_hkl_checksum              66511
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
_publcif_funding_html
;
;